LMucko/crystallography-open-database huggingface dataset:
Vanadyl dihydrogenoarsenate, VO(H2AsO4)2 : crystal structure and superexchange pathways
Amoros, P.; Beltran-Porter, A.; Villeneuve, G.; Beltran-Porter, D.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 257–272; doi:

data_4030420
_publ_section_title
;
 Vanadyl dihydrogenoarsenate, VO(H2AsO4)2 : crystal structure and
 superexchange pathways
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              257
_journal_page_last               272
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'As2 H4 O9 V'
_chemical_formula_weight         348.81
_space_group_IT_number           130
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      130
_symmetry_space_group_name_Hall  '-P 4a 2ac'
_symmetry_space_group_name_H-M   'P 4/n c c :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.1363(4)
_cell_length_b                   9.1363(4)
_cell_length_c                   8.1492(5)
_cell_volume                     680.23(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.542
_exptl_absorpt_coefficient_mu    23.415
_exptl_crystal_density_diffrn    3.406
_exptl_crystal_F_000             660
_pd_proc_ls_prof_R_factor        0.0694
_pd_proc_ls_prof_wR_factor       0.0796
_refine_ls_number_reflns         586
_refine_ls_R_I_factor            0.0408
_cod_data_source_file            EJSSIC-1992-29-257-272.cif
_cod_data_source_block           VO(H2AsO4)2
_cod_original_cell_volume        680.23(7)
_cod_original_sg_symbol_H-M      'P 4/n c c'
_cod_original_formula_sum        'H4 As2 O9 V'
_cod_database_code               4030420
The neutron crystal structure of the saccharinate complex [Cu(C7H4NO3S)2(H2O)4].2H2O
Cotton, F.A.; Falvello, L.R.; Murillo, C.A.; Schultz, A.J.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 311–320; doi:

data_4030421
_publ_section_title
;
 The neutron crystal structure of the saccharinate complex
 [Cu(C7H4NO3S)2(H2O)4].2H2O
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              311
_journal_page_last               320
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'C14 H20 Cu N2 O12 S2'
_chemical_formula_weight         536.01
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 101.19(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.208(2)
_cell_length_b                   16.146(4)
_cell_length_c                   7.161(2)
_cell_volume                     931.0(4)
_diffrn_ambient_temperature      15
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           white
_exptl_absorpt_coefficient_mu    1.497
_exptl_crystal_density_diffrn    1.912
_refine_ls_goodness_of_fit_all   1.101
_refine_ls_number_parameters     182
_refine_ls_number_reflns         2900
_refine_ls_R_factor_gt           0.047
_refine_ls_R_I_factor            0.083
_refine_ls_wR_factor_gt          0.094
_cod_data_source_file            EJSSIC-1992-29-311-320.cif
_cod_data_source_block           saccharinate-Cu-complex
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4030421
Synthesis of the new ternary intermetallic phase Li38(GaxZn1-x)101 x=0.663, displaying a hexagonal crystal superstucture. Structural approach in the subcell unit
Tillard-Charbonnel, M.; Chouaibi, N.; Belin, C.; Lapasset, J.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 347–359; doi:

data_4030422
_publ_section_title
;
 Synthesis of the new ternary intermetallic phase Li38(GaxZn1-x)101
 x=0.663, displaying a hexagonal crystal superstucture. Structural
 approach in the subcell unit
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              347
_journal_page_last               359
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Ga67 Li38 Zn34'
_chemical_formula_weight         7159.1
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   14.174(3)
_cell_length_b                   14.174(3)
_cell_length_c                   13.535(2)
_cell_volume                     2354.9(8)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    27.51
_exptl_crystal_density_diffrn    5.099
_refine_ls_number_reflns         575
_refine_ls_R_factor_gt           0.0543
_refine_ls_wR_factor_gt          0.0521
_cod_data_source_file            EJSSIC-1992-29-347-359.cif
_cod_data_source_block           Li38
_cod_original_cell_volume        2354.9(12)
_cod_database_code               4030422
Structure of the gamma' form of copper (II) quinolinolate and structural filiations to related M2+ complexes
Ammor, S.; Coquerel, G.; Perez, G.; Robert, F.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 445–453; doi:

data_4030423
_publ_section_title
;
 Structure of the gamma' form of copper (II) quinolinolate and structural
 filiations to related M2+ complexes
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              445
_journal_page_last               453
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'C18 H12 Cu N2 O2'
_chemical_formula_weight         351.85
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 120.48(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.213(2)
_cell_length_b                   5.075(1)
_cell_length_c                   15.325(2)
_cell_volume                     684.5(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    1.607
_exptl_crystal_density_diffrn    1.707
_exptl_crystal_F_000             358
_refine_ls_number_reflns         855
_refine_ls_R_factor_gt           0.04
_cod_data_source_file            EJSSIC-1992-29-445-453.cif
_cod_data_source_block           copper-quinolinolate
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4030423
Structural aspects of the metal-insulator transition in BaPb(1-x)TlxO(3-x/2) by neutron diffraction
Greedan, J.E.; Willmer, K.L.; Gibbs, H.F.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 505–518; doi:

data_4030424
_publ_section_title
;
 Structural aspects of the metal-insulator transition in
 BaPb(1-x)TlxO(3-x/2) by neutron diffraction
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              505
_journal_page_last               518
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Ba O2.9 Pb0.8 Tl0.2'
_chemical_formula_weight         390.36
_space_group_IT_number           74
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.0406(25)
_cell_length_b                   8.5449(42)
_cell_length_c                   6.0558(19)
_cell_volume                     312.6(2)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.3915
_exptl_crystal_density_diffrn    8.262
_pd_proc_ls_prof_wR_expected     0.0287
_pd_proc_ls_prof_wR_factor       0.0635
_refine_ls_R_I_factor            0.0804
_cod_data_source_file            EJSSIC-1992-29-505-518-1.cif
_cod_data_source_block           BaPb(1-x)TlxO(3-x/2)-I
_cod_database_code               4030424
Structural aspects of the metal-insulator transition in BaPb(1-x)TlxO(3-x/2) by neutron diffraction
Greedan, J.E.; Willmer, K.L.; Gibbs, H.F.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 505–518; doi:

data_4030425
_publ_section_title
;
 Structural aspects of the metal-insulator transition in
 BaPb(1-x)TlxO(3-x/2) by neutron diffraction
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              505
_journal_page_last               518
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Ba O2.65 Pb0.3 Tl0.7'
_chemical_formula_weight         384.95
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.0871(36)
_cell_length_b                   17.2719(56)
_cell_length_c                   6.1285(35)
_cell_volume                     644.3(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.3915
_exptl_crystal_density_diffrn    7.888
_pd_proc_ls_prof_wR_expected     0.0282
_pd_proc_ls_prof_wR_factor       0.0526
_refine_ls_R_I_factor            0.0960
_cod_data_source_file            EJSSIC-1992-29-505-518-2.cif
_cod_data_source_block           BaPb(1-x)TlxO(3-x/2)-II
_cod_database_code               4030425
Structural aspects of the metal-insulator transition in BaPb(1-x)TlxO(3-x/2) by neutron diffraction
Greedan, J.E.; Willmer, K.L.; Gibbs, H.F.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 505–518; doi:

data_4030426
_publ_section_title
;
 Structural aspects of the metal-insulator transition in
 BaPb(1-x)TlxO(3-x/2) by neutron diffraction
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              505
_journal_page_last               518
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Ba O2.6 Pb0.2 Tl0.8'
_chemical_formula_weight         383.87
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.0896(34)
_cell_length_b                   17.2726(86)
_cell_length_c                   6.1463(40)
_cell_volume                     646.5(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.3915
_exptl_crystal_density_diffrn    7.855
_pd_proc_ls_prof_wR_expected     0.0292
_pd_proc_ls_prof_wR_factor       0.0510
_refine_ls_R_I_factor            0.0659
_cod_data_source_file            EJSSIC-1992-29-505-518-3.cif
_cod_data_source_block           BaPb(1-x)TlxO(3-x/2)-III
_cod_database_code               4030426
Structural aspects of the metal-insulator transition in BaPb(1-x)TlxO(3-x/2) by neutron diffraction
Greedan, J.E.; Willmer, K.L.; Gibbs, H.F.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 505–518; doi:

data_4030427
_publ_section_title
;
 Structural aspects of the metal-insulator transition in
 BaPb(1-x)TlxO(3-x/2) by neutron diffraction
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              505
_journal_page_last               518
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Ba O2.55 Pb0.1 Tl0.9'
_chemical_formula_weight         382.79
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   6.0873(24)
_cell_length_b                   17.2696(60)
_cell_length_c                   6.2372(28)
_cell_volume                     655.7(5)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.3915
_exptl_crystal_density_diffrn    7.739
_pd_proc_ls_prof_wR_expected     0.0209
_pd_proc_ls_prof_wR_factor       0.0523
_refine_ls_R_I_factor            0.0805
_cod_data_source_file            EJSSIC-1992-29-505-518-4.cif
_cod_data_source_block           BaPb(1-x)TlxO(3-x/2)-IV
_cod_original_cell_volume        655.7(4)
_cod_database_code               4030427
Preparation and crystal structure of the phosphato-niobate Tl3NaNb4O9(PO4)2
Fakhfakh, M.; Verbaere, A.; Jouini, N.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 563–572; doi:

data_4030428
_publ_section_title
;
 Preparation and crystal structure of the phosphato-niobate
 Tl3NaNb4O9(PO4)2
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              563
_journal_page_last               572
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Na Nb4 O17 P2 Tl3'
_chemical_formula_weight         1341.71
_space_group_IT_number           40
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      40
_symmetry_space_group_name_Hall  'C -2c 2'
_symmetry_space_group_name_H-M   'C 2 c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.891(1)
_cell_length_b                   21.298(2)
_cell_length_c                   7.346(1)
_cell_volume                     1547.5(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    34.303
_exptl_crystal_density_diffrn    5.759
_exptl_crystal_F_000             2336
_refine_ls_number_parameters     88
_refine_ls_number_reflns         788
_refine_ls_R_factor_gt           0.047
_refine_ls_wR_factor_gt          0.053
_cod_data_source_file            EJSSIC-1992-29-563-572.cif
_cod_data_source_block           Tl3NaNb4O9(PO4)2
_cod_database_code               4030428
Synthesis and crystal structure of a volatile molecular precursor of copper: [CuN(SiMe3)2]4
Miele, P.; Foulon, J.D.; Hovnanian, N.; Durand, J.; Cot, L.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 573–583; doi:

data_4030429
_publ_section_title
;
 Synthesis and crystal structure of a volatile molecular precursor of
 copper: [CuN(SiMe3)2]4
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              573
_journal_page_last               583
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'C24 H72 Cu4 N4 Si8'
_chemical_formula_weight         895.7
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-I 2y'
_symmetry_space_group_name_H-M   'I 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.065(14)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.3805(20)
_cell_length_b                   13.561(1)
_cell_length_c                   17.799(2)
_cell_volume                     2264.2(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    2.071
_exptl_crystal_density_diffrn    1.856
_exptl_crystal_F_000             944
_refine_ls_number_parameters     99
_refine_ls_number_reflns         1958
_refine_ls_R_factor_gt           0.049
_refine_ls_wR_factor_gt          0.067
_cod_data_source_file            EJSSIC-1992-29-573-583.cif
_cod_data_source_block           CuN(SiMe3)2
_cod_original_sg_symbol_H-M      'I 2/m'
_cod_original_formula_sum        'C24 H72 N4 Si8 Cu4'
_cod_database_code               4030429
Single-crystal investigations on PtF4 and PtF5
Muller, B.G.; Serafin, M.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 625–633; doi:

data_4030430
_publ_section_title
;
 Single-crystal investigations on PtF4 and PtF5
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              625
_journal_page_last               633
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'F4 Pt'
_chemical_formula_weight         271.08
_space_group_IT_number           43
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      43
_symmetry_space_group_name_Hall  'F 2 -2d'
_symmetry_space_group_name_H-M   'F d d 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   9.590(6)
_cell_length_b                   9.284(6)
_cell_length_c                   5.712(3)
_cell_volume                     508.6(5)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           AgK\a
_diffrn_radiation_wavelength     0.5609
_exptl_absorpt_coefficient_mu    29.903
_exptl_crystal_density_diffrn    7.081
_exptl_crystal_F_000             912
_refine_ls_number_parameters     24
_refine_ls_number_reflns         279
_refine_ls_R_factor_gt           0.042
_refine_ls_wR_factor_gt          0.031
_cod_data_source_file            EJSSIC-1992-29-625-633-1.cif
_cod_data_source_block           PtF4
_cod_database_code               4030430
Single-crystal investigations on PtF4 and PtF5
Muller, B.G.; Serafin, M.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 625–633; doi:

data_4030431
_publ_section_title
;
 Single-crystal investigations on PtF4 and PtF5
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              625
_journal_page_last               633
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'F5 Pt'
_chemical_formula_weight         290.076
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.98(4)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   5.523(3)
_cell_length_b                   9.942(6)
_cell_length_c                   12.430(6)
_cell_volume                     672.2(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_exptl_absorpt_coefficient_mu    41.723
_exptl_crystal_density_diffrn    5.733
_exptl_crystal_F_000             984
_refine_ls_number_parameters     110
_refine_ls_number_reflns         1401
_refine_ls_R_factor_gt           0.063
_refine_ls_wR_factor_gt          0.045
_cod_data_source_file            EJSSIC-1992-29-625-633-2.cif
_cod_data_source_block           PtF5
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4030431
Iodine pentafluoride-hydrogen fluoride co-crystallisates, directed weak interactions
Mahjoub, A.R.; Leopold, D.; Seppelt, K.; European Journal of Solid State and Inorganic Chemistry 29 (1992) 635–647; doi:

data_4030432
_publ_section_title
;
 Iodine pentafluoride-hydrogen fluoride co-crystallisates, directed weak
 interactions
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              635
_journal_page_last               647
_journal_volume                  29
_journal_year                    1992
_chemical_formula_sum            'Cs F7 H I'
_chemical_formula_weight         393.82
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                109.25(4)
_cell_angle_beta                 106.81(4)
_cell_angle_gamma                92.15(4)
_cell_formula_units_Z            2
_cell_length_a                   5.303(2)
_cell_length_b                   8.163(4)
_cell_length_c                   8.437(4)
_cell_volume                     326.5(3)
_diffrn_ambient_temperature      120
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    10.457
_exptl_crystal_density_diffrn    4.006
_exptl_crystal_F_000             344
_refine_ls_number_parameters     82
_refine_ls_number_reflns         1728
_refine_ls_R_factor_gt           0.032
_refine_ls_wR_factor_gt          0.034
_cod_data_source_file            EJSSIC-1992-29-635-647-1.cif
_cod_data_source_block           1
_cod_original_formula_sum        'H Cs F7 I'
_cod_database_code               4030432